Optical alignment of oval graphene flakes E. M OBINI1,* , A. R AHIMZADEGAN2 , R. A LAEE2,3 ,
C. R OCKSTUHL2,4
Center of Photonics, Friedrich-Schiller University, Jena, Germany of Theoretical Solid State Physics, Karlsruhe Institute of Technology, Karlsruhe, Germany 3 Max Planck Institute for the Science of Light, Erlangen, Germany 4 Institute of Nanotechnology, Karlsruhe Institute of Technology, Karlsruhe, Germany * Corresponding author: [email protected]
Compiled February 7, 2017
Patterned graphene, as an atomically thin layer, supports localized surface plasmon-polaritons (LSPPs) at mid-infrared or far-infrared frequencies. This provides a pronounced optical force/torque in addition to large optical cross sections and will make it an ideal candidate for optical manipulation. Here, we study the optical force and torque exerted by a linearly polarized plane wave on circular and oval graphene flakes. Whereas the torque vanishes for circular flakes, the finite torque allows rotating and orienting oval flakes relative to the electric field polarization. Depending on the wavelength, the alignment is either perpendicular or parallel. In our contribution, we rely on full-wave numerical simulation but also on an analytical model that treats the graphene flakes in dipole approximation. The presented results reveal a good level of control on the spatial alignment of graphene flakes subjected to far-infrared illumination. © 2017 Optical Society of America
als , trapping of micro/nano entities , manipulating of dielectric particles , or optomechanical manipulation . Here, we study oval graphene flakes that, in contrast to circular graphene flakes, owing to their in-plane anisotropy, can be rotated by linearly polarized light. They can be aligned either parallel or perpendicular to the incident electric field vector, depending on the frequency of operation. The misalignment angle φ between the incident electric field and the major oval axis (here + x) can be tuned to control direction and magnitude of the exerted torque. This torque allows to align flakes upon request (Fig. 1).
OCIS codes: (290.5855) Scattering, polarization; (260.5430) Polarization (250.5403) Plasmonics.
Graphene, a two dimensional crystal of carbon atoms arranged in a honeycomb pattern, exhibits intriguing photonic and electronic properties [1, 2]. Dynamical tuning of the conductivity via gate voltage or chemical doping , a tunable bandgap via electrical gating [4, 5], a higher level of light confinement compared to plasmonic materials [6–8], and a high ratio of extinction cross section to the geometrical cross section  are a few to mention. Among the aforementioned properties, it is most notably the possibility to enhance the light-matter interaction that provides enough motivation to consider graphene in various photonic applications. To observe a resonant light-matter interaction one requires to nano and/or micro pattern graphene with suitable shapes, e.g. ribbons [10–12] or disks  such that it sustains localized surface plasmon polaritons. Applications emerging from the enhanced light-matter interaction would additionally benefit from the ability to optically manipulate the spatial position, arrangement, and orientation of the graphene flakes on demand comparable to conventional plasmonic particles [13–15, 17]. Examples for such applications are optically reconfigurable materi-
Linear polarization: N=0
Linear polarization: N≠ 0
Fig. 1. Main idea of our work: A linearly polarized plane wave
can align and rotate an oval graphene flake. The figures on the left and right show the schematic of a circular graphene (in-plane isotropic) flake and an oval graphene (in-plane anisotropic) flake, respectively. Both are illuminated by a linearly polarized plane wave propagating in the +z direction, perpendicular to the flake plane. The red arrow shows the electric field vector of the illuminating light on the flake plane. In the following, we employ three approaches to calculate the polarizability, the optical cross section and the optical force and torque. Not each of these method is applied to each sub-aspect; but all together they provide a solid methodological framework to explore the properties of the pertinent system. In the first approach, we study the full-wave dynamics in the entire setup. This requires to solve Maxwell’s equations numerically. We use a finite element method (FEM) for this purpose . The simulated fields are used to calculate the Maxwell’s stress tensor (MST) from which eventually the force
and torque as expressed in Eqs. 1- 3 can be calculated. The results of this approach are exact. In the second approach (semi-analytic force and torque), we assume that the graphene flake possesses only an electric dipole response. This allows to use existing analytical expressions for the force and toque as expressed in Eqs. 5- 9. The approach is semi-analytic since a multipole expansion of the numerically simulated induced electric current density [22, 23] is used to extract the electric dipole moment of the graphene flake. In a third approach, in addition analytical expressions for the polarizability of the graphene flakes are used to compute the induced force and toque (quasi-static approximation). The agreement of the predictable force and torque with the different methods is assessed. All calculations consider the graphene flakes to be in air. The electromagnetic quantities in phasor form have a time dependency of exp(−iωt). Quantities in time domain are denoted by an underline. The time averaged mechanical force exerted on an arbitrary particle by an optical wave is calculated as [22, 24]: I = F= T(r, t) · n dS , (1) S
where S is any closed surface surrounding the particle, n is a =
unit vector that points outward, and T is the Maxwell’s stress tensor. The Maxwell’s stress tensor is a tensor of second rank whose components can be calculated as [22, 24]: 1 T ij = ε 0 Ei E j + c2 Bi B j − δij |E|2 + |B|2 , (2) 2 in which E and B are the total (incident and scattered) electric and magnetic fields in the i, j = x, y, z coordinates; and δij is the Kronecker delta function. The time averaged optical torque on an arbitrary particle by an optical wave can be calculated as: I = (3) N=− n · T(r, t) × r dS . S
This approach provides exact solutions but it complicates the physical discussion. To entail such discussion, we also apply a multipole expansion method, to expanded the induced current density in the graphene flakes into elementary multipole moments. The link between the incident field and the induced multipole moments is given by polarizability tensors. For the oval graphene flake, that have a wavelength much longer than the size of the flakes, we can restrict our attention in good approximation to the electric dipole polarizability. The electric dipole in-plane polarizabilities of the flake can be expressed as: =
α = αk e x e x + α⊥ ey ey ,
with αk and α⊥ being the in-plane x (parallel to the flake major axis) and y (perpendicular to the flake major axis) polarizabilities, respectively. For an electric dipolar particle (i.e. a particle with only a nonnegligible electric dipole response) illuminated with an arbitrary illumination, the induced optical force reads as [25–29]: Fp = =
1 λ2 , to the field polarization. The torque caused by the optical field attempts to minimize the potential energy of the object. Assuming the graphene flake is a dipolar particle, as noted above, its potential energy in terms of the induced dipole moment, D E U = − hp · Ei, can be reduced to − hp⊥ · Ei and − pk · E around λ1 and λ2 , respectively. Depending on the sign of these perpendicular and parallel polarizabilities, the torque directs the object towards the lower energy configuration i.e. parallel or perpendicular to the electric field. The optical force and torque at λ = λ1 and λ = λ2 as a function of φ are illustrated in Fig. 4, showing that the exerted force and torque can be extended and modified by altering the incident field polarization. In conclusion, we studied the exerted optical force and torque on an oval graphene flake and we demonstrated theoretically the possibility of its alignment and rotation by a linearly polarized plane wave illumination. Our findings show that for a specific oval graphene flake of particular size, by altering the Fermi energy, incident light wavelength and changing the misalignment angle (φ), a good level of control on the direction and magnitude of rotation of the object is possible. This in turn allow us to achieve a tunable light manipulation of small size
REFERENCES 1. K. Novoselov, A. K. Geim, S. Morozov, D. Jiang, M. Katsnelson, I. Grigorieva, S. Dubonos, and A. Firsov, Nature 438, 197 (2005). 2. K. S. Novoselov, A. K. Geim, S. V. Morozov, D. Jiang, Y. Zhang, S. V. Dubonos, I. V. Grigorieva, and A. A. Firsov, Science 306, 666 (2004). 3. A. Vakil and N. Engheta, Science 332, 1291 (2011). 4. F. Wang, Y. Zhang, C. Tian, C. Girit, A. Zettl, M. Crommie, and Y. R. Shen, Science 320, 206 (2008). 5. Y. Zhang, T.-T. Tang, C. Girit, Z. Hao, M. C. Martin, A. Zettl, M. F. Crommie, Y. R. Shen, and F. Wang, Nature 459, 820 (2009). 6. M. Jablan, H. Buljan, and M. Soljaˇci´c, Phys. Rev. B 80, 245435 (2009). 7. S. Mikhailov and K. Ziegler, Phys. Rev. Lett. 99, 016803 (2007). 8. E. Hwang and S. D. Sarma, Phys. Rev. B 75, 205418 (2007). 9. S. Thongrattanasiri, F. H. Koppens, and F. J. G. de Abajo, Phys. Rev. Lett. 108, 047401 (2012). 10. Z. Fei, M. Goldflam, J.-S. Wu, S. Dai, M. Wagner, A. McLeod, M. Liu, K. Post, S. Zhu, G. Janssen et al., Nano lett. 15, 8271 (2015). 11. J. R. Piper and S. Fan, ACS Photonics 1, 347 (2014). 12. R. Alaee, M. Farhat, C. Rockstuhl, and F. Lederer, Opt. Express 20, 28017 (2012). 13. L. Tong, V. D. Miljkovic, and M. Käll, Nano lett. 10, 268 (2009). 14. X. Xu, C. Cheng, Y. Zhang, H. Lei, and B. Li, J. Phys. Chem. Lett. 7, 314 (2016). 15. R. A. Nome, M. J. Guffey, N. F. Scherer, and S. K. Gray, J. Phys. Chem. A 113, 4408 (2009). 16. C. W. Twombly, J. S. Evans, and I. I. Smalyukh, Opt. Express 21, 1324 (2013). 17. M. L. Juan, M. Righini and R. Quidant, Nat. Photon. 5, 349 (2011). 18. J. Zhang, W. Liu, Z. Zhu, X. Yuan and S. Qin, Sci. Rep. 6, (2016). 19. Y. Yang, Z. Shi, J. Li, and Z.-Y. Li, Photonics Research 4, 65 (2016). 20. S. H. Mousavi, P. T. Rakich, and Z. Wang, ACS Photonics 1, 1107 (2014). 21. See www.comsol.com for the details of computational modeling. 22. J. D. Jackson, Classical electrodynamics (Wiley, 1999). 23. I. Fernandez-Corbaton, S. Nanz, R. Alaee, and C. Rockstuhl, Opt. Express 23, 33044 (2015). 24. L. Novotny and B. Hecht, Principles of nano-optics (Cambridge university press, 2012). 25. P. Chaumet and M. Nieto-Vesperinas, Opt. lett. 25, 1065 (2000). 26. M. Nieto-Vesperinas, Opt. Lett. 40, 3021 (2015). 27. J. Chen, J. Ng, Z. Lin, and C. Chan, Nat. Photon. 5, 531 (2011). 28. V. Gusynin, S. Sharapov, and J. Carbotte, J. Phys. Condens. Matter 19, 026222 (2006). 29. A. Rahimzadegan, M. Fruhnert, R. Alaee, I. Fernandez-Corbaton, and C. Rockstuhl, Phys. Rev. B 94, 125123 (2016). 30. A. Rahimzadegan, R. Alaee, I. Fernandez-Corbaton, and C. Rockstuhl, arXiv preprint arXiv:1605.03945 (2016). 31. L. Falkovsky and S. Pershoguba, Phys. Rev. B 76, 153410 (2007). 32. G. W. Hanson, Journal of Applied Physics 103, 064302 (2008). 33. F. J. G. de Abajo and A. Manjavacas, Faraday discussions 178, 87 (2015). 34. F. J. Garcia de Abajo, ACS Nano 7, 11409 (2013). 35. F. J. Garcia de Abajo, ACS Photonics 1, 135 (2014). 36. C. F. Bohren and D. R. Huffman, Absorption and scattering of light by small particles (John Wiley & Sons, 2008). 37. L. D. Landau, J. Bell, M. Kearsley, L. Pitaevskii, E. Lifshitz, and J. Sykes, Electrodynamics of continuous mediaflake, vol. 8 (elsevier, 2013).
INFORMATIONAL FIFTH PAGE REFERENCES 1. K. Novoselov, A. K. Geim, S. Morozov, D. Jiang, M. Katsnelson, I. Grigorieva, S. Dubonos, and A. Firsov, “Two-dimensional gas of massless dirac fermions in graphene,” , Nature, vol. 438, no. 7065, pp. 197–200, 2005. 2. K. S. Novoselov, A. K. Geim, S. V. Morozov, D. Jiang, Y. Zhang, S. V. Dubonos, I. V. Grigorieva, and A. A. Firsov, “Electric field effect in atomically thin carbon films,” , Science, vol. 306, no. 5696, pp. 666– 669, 2004. 3. A. Vakil and N. Engheta, “Transformation optics using graphene,” , Science, vol. 332, no. 6035, pp. 1291–1294, 2011. 4. F. Wang, Y. Zhang, C. Tian, C. Girit, A. Zettl, M. Crommie, and Y. R. Shen, “Gate-variable optical transitions in graphene,” , Science, vol. 320, no. 5873, pp. 206–209, 2008. 5. Y. Zhang, T.-T. Tang, C. Girit, Z. Hao, M. C. Martin, A. Zettl, M. F. Crommie, Y. R. Shen, and F. Wang, “Direct observation of a widely tunable bandgap in bilayer graphene,” , Nature, vol. 459, no. 7248, pp. 820–823, 2009. 6. M. Jablan, H. Buljan, and M. Soljaˇci´c, “Plasmonics in graphene at infrared frequencies,” , Phys. Rev. B, vol. 80, no. 24, p. 245435, 2009. 7. S. Mikhailov and K. Ziegler, “New electromagnetic mode in graphene,” , Phys. Rev. Lett., vol. 99, no. 1, p. 016803, 2007. 8. E. Hwang and S. D. Sarma, “Dielectric function, screening, and plasmons in two-dimensional graphene,” , Phys. Rev. B, vol. 75, no. 20, p. 205418, 2007. 9. S. Thongrattanasiri, F. H. Koppens, and F. J. G. de Abajo, “Complete optical absorption in periodically patterned graphene,” , Phys. Rev. Lett., vol. 108, no. 4, p. 047401, 2012. 10. Z. Fei, M. Goldflam, J.-S. Wu, S. Dai, M. Wagner, A. McLeod, M. Liu, K. Post, S. Zhu, G. Janssen, et al., “Edge and surface plasmons in graphene nanoribbons,” , Nano lett., vol. 15, no. 12, pp. 8271–8276, 2015. 11. J. R. Piper and S. Fan, “Total absorption in a graphene monolayer in the optical regime by critical coupling with a photonic crystal guided resonance,” , ACS Photonics, vol. 1, no. 4, pp. 347–353, 2014. 12. R. Alaee, M. Farhat, C. Rockstuhl, and F. Lederer, “A perfect absorber made of a graphene micro-ribbon metamaterial,” , Opt. Express, vol. 20, pp. 28017–28024, Dec 2012. 13. L. Tong, V. D. Miljkovic, and M. Käll, “Alignment, rotation, and spinning of single plasmonic nanoparticles and nanowires using polarization dependent optical forces,” , Nano lett., vol. 10, no. 1, pp. 268–273, 2009. 14. X. Xu, C. Cheng, Y. Zhang, H. Lei, and B. Li, “Scattering and extinction torques: How plasmon resonances affect the orientation behavior of a nanorod in linearly polarized light,” , J. Phys. Chem. Lett., vol. 7, no. 2, pp. 314–319, 2016. 15. R. A. Nome, M. J. Guffey, N. F. Scherer, and S. K. Gray, “Plasmonic interactions and optical forces between au bipyramidal nanoparticle dimersï¿½,” , J. Phys. Chem. A, vol. 113, no. 16, pp. 4408–4415, 2009. 16. C. W. Twombly, J. S. Evans, and I. I. Smalyukh, “Optical manipulation of self-aligned graphene flakes in liquid crystals,” , Opt. Express, vol. 21, no. 1, pp. 1324–1334, 2013. 17. M. L. Juan, M. Righini, and R. Quidant, “Plasmon nano-optical tweezers,” , Nat Photon, vol. 5, pp. 349–356, June 2011. 18. J. Zhang, W. Liu, Z. Zhu, X. Yuan and S. Qin, “Towards nano-optical tweezers with graphene plasmons: Numerical investigation of trapping 10-nm particles with mid-infrared light,” Sci. Rep. 6, (2016). 19. Y. Yang, Z. Shi, J. Li, and Z.-Y. Li, “Optical forces exerted on a graphenecoated dielectric particle by a focused gaussian beam,” Photonics Research, vol. 4, no. 2, pp. 65–69, 2016. 20. S. H. Mousavi, P. T. Rakich, and Z. Wang, “Strong thz and infrared optical forces on a suspended single-layer graphene sheet,” , ACS Photonics, vol. 1, no. 11, pp. 1107–1115, 2014. 21. C. Multiphysics, “See www.comsol.com for the details of computational modeling.,” 2012. 22. J. D. Jackson, Classical electrodynamics. Wiley, 1999.
23. I. Fernandez-Corbaton, S. Nanz, R. Alaee, and C. Rockstuhl, “Exact dipolar moments of a localized electric current distribution,” , Opt. Express, vol. 23, no. 26, pp. 33044–33064, 2015. 24. L. Novotny and B. Hecht, Principles of nano-optics. Cambridge university press, 2012. 25. P. Chaumet and M. Nieto-Vesperinas, “Time-averaged total force on a dipolar sphere in an electromagnetic field,” , Opt. lett., vol. 25, no. 15, pp. 1065–1067, 2000. 26. M. Nieto-Vesperinas, “Optical torque on small bi-isotropic particles,” , Opt. Lett., vol. 40, no. 13, pp. 3021–3024, 2015. 27. J. Chen, J. Ng, Z. Lin, and C. Chan, “Optical pulling force,” , Nat. Photon., vol. 5, no. 9, pp. 531–534, 2011. 28. V. Gusynin, S. Sharapov, and J. Carbotte, “Magneto-optical conductivity in graphene,” , J. Phys. Condens. Matter, vol. 19, no. 2, p. 026222, 2006. 29. A. Rahimzadegan, M. Fruhnert, R. Alaee, I. Fernandez-Corbaton, and C. Rockstuhl, “Optical force and torque on dipolar dual chiral particles,” , Phys. Rev. B, vol. 94, p. 125123, Sep 2016. 30. A. Rahimzadegan, R. Alaee, I. Fernandez-Corbaton, and C. Rockstuhl, “Fundamental limits of optical force and torque,” , arXiv preprint arXiv:1605.03945, 2016. 31. L. Falkovsky and S. Pershoguba, “Optical far-infrared properties of a graphene monolayer and multilayer,” , Phys. Rev. B, vol. 76, no. 15, p. 153410, 2007. 32. G. W. Hanson, “Dyadic greens functions and guided surface waves for a surface conductivity model of graphene,” , Journal of Applied Physics, vol. 103, no. 6, p. 064302, 2008. 33. F. J. G. de Abajo and A. Manjavacas, “Plasmonics in atomically thin materials,” , Faraday discussions, vol. 178, pp. 87–107, 2015. 34. F. J. Garcia de Abajo, “Multiple excitation of confined graphene plasmons by single free electrons,” , ACS Nano, vol. 7, no. 12, pp. 11409– 11419, 2013. 35. F. J. Garcia de Abajo, “Graphene plasmonics: challenges and opportunities,” , ACS Photonics, vol. 1, no. 3, pp. 135–152, 2014. 36. C. F. Bohren and D. R. Huffman, Absorption and scattering of light by small particles. John Wiley & Sons, 2008. 37. L. D. Landau, J. Bell, M. Kearsley, L. Pitaevskii, E. Lifshitz, and J. Sykes, Electrodynamics of continuous mediaflake, vol. 8. elsevier, 2013.